Maskell, D., Heath, A. and Walker, P. (2013) Laboratory scale testing of extruded earth masonry units. Materials & Design, 45. pp. 359-364. ISSN 0261-3069
Link to official URL (if available): http://dx.doi.org/10.1016/j.matdes.2012.09.008
Opus: University of Bath Online Publication Store
This version is made available in accordance with publisher policies. Please cite only the published version using the reference above.
See http://opus.bath.ac.uk/ for usage policies.
Please scroll down to view the document.
Laboratory Scale Testing of Extruded Earth Masonry Units
Daniel Maskell(a), Andrew Heath(a) and Pete Walker(a)
(a)BRE Centre for Innovative Construction Materials Department of Architecture and Civil Engineering University of Bath Bath BA2 7AY
Daniel Maskell BRE Centre for Innovative Construction Materials Department of Architecture and Civil Engineering University of Bath Bath BA2 7AY
There has been a resurgence in use of earth as a construction material largely driven by environmental concerns. Extruded earth masonry is a method of earth brick production that utilises existing fired brick manufacturing techniques. Extruded earth has distinct physical characteristics compared to other earthen building techniques. As industrial scale extrusion trials require large volumes of material, laboratory scale material development relies on samples prepared using alternative forming methods, such as moulding and compaction, which do not reliably reproduce the full-scale manufacturing process. The paper presents a representative method of manufacturing small scale extruded earth bricks. A suitable testing methodology is proposed, with varying curing conditions investigated. The small scale bricks are compared against equivalent large scale unfired earth bricks. The small scale bricks achieved a compressive strength of 3.39MPa and with a corrected difference compared to the full scale bricks of 0.07MPa; were found to be a reliable basis for laboratory scale investigation of material performance. The relationship that describes the effect of moisture content on strength exists for both small and large scale bricks.
Masonry; Earth Construction; Compressive Strength Testing; Size Effect
Earth as a construction material is one of the oldest and the most common building materials still in use . Earth architecture is commonly associated with developing countries and within the UK the heritage of earth construction largely ended during the 19th Century .
There has been a resurgence of construction with earth largely due to environmental concerns of high embodied energy and the global warming potential of fired bricks and cement based products . While rammed earth has shown the potential for contemporary earthen architecture, greater impacts are likely to come from earth masonry where current building practices can be easily adopted.
Compressed Earth Blocks (CEB) are masonry units that are manufactured by manually or mechanically compressing earth within a mould. A growing body of research has focused on the strength and durability of CEB [4,5]. While Jayasinghe and Mallawaarachchi  and Oti et al.  showed the potential for CEB to be produced on an industrial scale, Heath et al.  showed the structural potential for commercially extruded bricks to remain unfired.
The manufacturing process of fired clay bricks prior to firing is also suitable, without any significant modification, for the production of unfired earth bricks. There is minimal additional capital cost of production due to an identical process being utilised and a reduced running cost due to economy of scale factors. Morton et al.  showed that by not firing the bricks 86% of the embodied energy of a fired brick could be saved. The commercial extrusion allows for a greater control over quality and reduced unit costs compared to CEB.
There has been limited research on the strength of unfired extruded masonry units with the exception of Heath et al. [7,9]. This is in part due to complexities of laboratory scale testing of extruded bricks. A suitable method of production and testing of extruded earth masonry units must be developed to allow for further research and development of unfired extruded earth masonry on a commercial scale.
Small scale masonry testing has been used for decades due to problems of full scale testing [10,11]. This approach is typically used to assess and investigate strengthening of existing structures as well as investigating the effects of extreme climatic events such as earthquakes. Testing at small scales is performed because of the cost and repeatability of undertaking full-scale tests .
This paper discusses how reduced laboratory scale brick manufacture can replicate full-scale production properties of extruded earth bricks. The focus will be on a suitable compressive strength testing methodology for small scale earth bricks, including the comparison to equivalent full scale bricks.
2 Materials and Methods
2.1 Materials A soil used for commercial fired brick manufacturing was selected. Heath et al.  established that fired brick soils are also suitable for unfired clay bricks. Identical soil was used for both the full scale and small scale bricks without any modification or scaling. The soils can be described as a dark brown sandy SILT with a plasticity classification of a low plasticity clay . The physical properties and particle grading was determined by the methodology provided by BS 1377-2:1990 , with the mineralogical content of the soil determined by XRD; shown with the plasticity and particle size distribution in Table 1.
Table 1: Soil Properties
Physical Properties Liquid Limit 24.1 Plasticity Index 8.3 Linear Shrinkage 5.7
Particle Grading Sand 33.1 Silt 45.5 Clay 15.9
Mineral Content Siderite 2 Hematite 3 Smectite 3 Chlorite 6 Illite 16 Kaolinite 31 Quartz 39
2.2 Sample Preparation
2.2.1 Full Scale Full-scale bricks were manufactured by a commercial brick manufacture following the same methodology typically used for fired bricks. Following extraction, the soil is crushed and milled to a size of 2mm in preparation of extrusion. The soil is mixed with water to approximately the plastic limit of the soil in a series of rotating augers. This soil is then extruded under a vacuum through a precisely machined die. This produces a stiff column of clay, as in Fig. 1, that is subsequently cut into single bricks.
The process of extruding earth is a different form of soil compaction that is likely to impart unique physical characteristics compared to other forms brick manufacturing and soil compaction techniques. Bricks with much higher densities than those produced by CEB are achieved . In addition there is potential for particle alignment due to the friction and the tapering of the extrusion.
Figure 1: Commercial Extruder
2.2.2 Small Scale Mohammed et al.  observed anisotropic effects when using scaled bricks cut from a larger bricks. In order to produce similar physical characteristics to the bricks manufactured at full scale, it was essential that a similar extrusion process be used. Scaled bricks were manufactured within a laboratory environment at The University of Bath, using a small scale vacuum extruder as shown in Fig. 2. It was unfeasible to manufacture full scale bricks using this extruder, therefore bricks at 1:3 linear scale, thus 1:27 volumetric scale were produced as shown in Fig. 3.
This machine creates a similar production process to full scale extruded bricks. Soil that has been pre-mixed with the required water content is fed in to a series of augers that help to homogenise the mixture. Under a vacuum of 50kPa the clay is effectively compacted by reducing the cross sectional area at the point of extrusion to 72 mm by 34 mm. This produces a column of soil that is then cut into 22mm thick bricks as in Fig. 3.
Figure 2: Vacuum extruder
Figure 3: Scaled brick specimens
2.3 Optimum Moisture Content The inherent strength of earth construction is dependent on the soil type, moisture content and dry density. The dry density can be increased through increasing the amount of compaction, which is equally dependent on the soil type and the moisture content during compaction.
Compaction curves for different soil types that account for varying moisture contents during compaction are well established with the Maximum Dry Density (MDD) and Optimum Moisture Content (OMC) dependent on the soil type, but also the
compaction energy and compaction method. To optimise the inherent structural properties by achieving the MDD by extruding at the OMC is essential. A compaction curve for the extruded soil was established and shown in Fig. 4. The values shown are averages of no less than 40 bricks with a 4.7% maximum Coefficient of Variation (CV) of dry density. This was compared to the modified proctor method that is typically used for determining the OMC for rammed earth and other field compacted soils.
The modified Proctor method has proven unsuitable for the determination of OMC for extrusion. The compaction based OMC is much lower than that required for extrusion, Fig. 4. Extruding at moisture contents below the plasticity limit resulted in notable cracking in the brick surface and further more extrusion was not possible at moisture contents less than 14%. The OMC for extrusion is therefore at the plasticity limit of 16%, with all future work extru